IS : 3370 ( Part I ) - 1965
CODE OF PRACTICE FOR CONCRETE
STRUCTURES FOR THE STORAGE
PART I GENERAL REQUIREMENTS
( Tenth Reprint AUGUST 1992 )
UDC 621’642 : 666’972
0 Copyright 1966
BUREAU OF INDIAN STANDARDS
MANAK BHAVAN, 9 BAHADUR SHAH ZAFAR MARG
NEW DELHI 110002
( Reaffirmed 1999 )
CODE OF PRACTICE FOR CQNCRETE
STRUCTURES FO,R THE STORAGE
PART I GENERAL REQUIREMENTS
Cement and Concrete &ctional Committee, BDC 2
SHBI I(. K. NAB~EZIAB
The Concrete Association of India, Bombay
SHBI N. H. MOEILE ( Alternak to
Shri K. K. Nambiar )
SHBI K. F. ~NTIA M. N. Dastur & Co ( Pvt ) Ltd, Calcutta
COL G. BENJAMIN Engineer-in-Chief’s Branch, Armv Headauarters
S~sr R. S. MEHANDRU ( Alternatc)~
SHBI P. S. BEATNA~A~ Bhakra & Beas Designs Organization, New Delhi
DB I. C. DOS M. Pam CUDDOU Central Water & Power Commission (Ministry of
SEXI Y. K. MTJBTHY ( Alternate)
Irrigation & Power )
SEBI N. D. D~BTAEY In personal capacity (Dutt Niwas, 27 Laburnam
Road, Bombay-7 )
SEEI N. G. DEWAN Central Public Works Department, New Delhi
2ND &ROLE (Alternate)
Da R. R. ,HA~IANC+ADI The Associated Cement Companies Ltd, Bombay
Saar: V. N. PA1 ( Aknats )
SEBI P. C. HAZBA Geological Survey of India, Calcutta
JOINT DIBE~OB STAXDABDS Research, Designs & Standards Organisation ( Minis-
try of Railways )
SHBI S. B. Josri~ S. B. Joshi & Co Ltd, Bombay
SHBI M. M. LAL
PBOBS. R. MEH~A
U. P. Government Cement Factory, Churk
Cen~l.$oad Research Instrtute ( CSIR ), New
DB R. K. GHOSH (Altemafe)
SERL S. N. MUKEBJI National Test House, Calcutta
Srutr N. ,C. SENQUPTA ( Alternate.)
SERI EBACIE A. NADI~~HAE Institution of Engineers ( India), Calcutta
SHSI C. B. PATEL National Buildings Organization ( Ministry of Works
SHRI R~BINDEB SIN~H ( Alternuts )
F’BOSG. S. RAYASWAMY Cent;Arkz;ilding Research Institute ( CSIR ),
SEBI M. G. TAMHANKAB ( Alternafe )
( Continuedon page 2
8UREAU OF INDIAN STANDARDS
MANAK BHAVAN, 9 BAHADUR SHAH ZAFAR MARG
NEW DELHI 110002
( Conlinucdfm )agc 1)
Saar T. N. S. RAO Gammon India Ltd, Bombay
Sam S. R. PINHEIRO ( Altema& )
REPRESENTATIVE Martin Burn Ltd, Calcutta
SEIU NIHAR CHANDRA ROY Dalmia Cement ( Bharat ) Ltd, Calcutta
SECRETABY Central Board of Irrigation & Power, New Delhi
DB BE. SUBBA~AJU Indian Roads Congress, New Delhi
SHBI J. M. TBEHAN Roads Wing, Ministry of Transport
SHRI N. H. KESWANI ( Alternate )
DE H. C. VISVLBVABVA, Director, BlS ( Ex-ofiio Member)
Deputy Director ( Civil Engg )
Soar: Y. R. TANEJA
Eatra AssistantDirector ( Civil Engg ), BIS
Concrete Subcommittee, BDC 2 : 2
SEXI S. B. JOEBI S. B. Joshi & Co Ltd, Bombay
SHBI N. H. BEAQWANANI Engineer-in-Chief’s Branch, Army Headquarters
DR I. C. DOS M. PAIS CUDDOO Central Water & Power Commission (Ministry of
Irrigation & Power )
SBRI Y. K. MUBTEY ( Altcrnafe )
DEPUTY DIRECTOR STANDARDS Research, Designs & Standards Organization
(B&S) ( Ministry of Railways )
DIBECTOB Engineering Research Department, Hyderabad
SHRI V. N. GUNAJI Maharashtra Public Works Department
SERI M. A. HAFEICZ National Buildings Organization ( Ministry of Works
SRRI B. S. SHIVAMUBTHY ( AI&mate )
SERI C. L. HANDA Central Water & Power Commission ( Ministry of
Irrigation & Power )
SBRI P. C. HAZRA Geological Survey of India, Calcutta
SERI K. K. NAMBIAB The Concrete Association of India, Bombay
SHRI ,C. L. N. IYEN~AB ( Alternate)
Da M. L. Puxr Cent.Jlhyd Research Institute ( CSIR), New
PROB G. S. RAYASWAE~Y Central Building Research Institute ( CSIR )
Sasr M. G. TAMHANXAR (Al¬e )
SHBI T. N, S. RAO Gammon India Ltd, Bombay
SHRI S. R. Praamso ( Alternufe )
S~JFERINTENDIN~ENOINEEB, 2ND Central Public Works Department, New Delhi
SHRI 0. P. GOEL (A&mate)
SBRI J. M. TREEAN Roads Wing, Ministry of Transport
SHRI R. P. SIKKA ( Alternate )
DR H. C. VISVESVARAYA Indian Standards Institution
SHRI H. T. YAN Brai$vvz:taBurn 6% Jessop Construction Co Ltd,
Panel for Concrete Codes, BDC 2 : 2 : 1
SERI S. B. JOSHI S. B. Joshi & Co Ltd, Bombay
SHRI K. K. NAMBIAR The Concrete Association of India, Bombav
DR H. C. VISVESVARAYA Indian Standards Institution
CODE OF PRACTICE FOR CONCRETE
STRUCTURES FOR THE STORAGE
PART I GENERAL REQUIREMENTS
0.1This Indian Standard ( Part I) was adopted by the Indian Standards
Institution on 19 November 1965, after the draft finalized by the
Cement and Concrete Sectional Committee had been approved by the
Civil Engineering Division Council.
0.2 The need for a code covering the design and construction of reinforced
concrete and prestressed concrete structures for the storage of liquids has
been long felt in this country. So far, such structures have been designed
to varying standards adapted from the recommendations of the Institution
of Civil Engineers and of the Portland Cement Association with ‘the result
that the resultant structures cannot be guaranteed to possess a uniform
safety margin and dependability. Moreover, the design and construction
methods in reinforced concrete and prestressed concrete are influenced by
the prevailing construction practices, the physical properties of the
materials and the climatic conditions. The need was, therefore, felt to lay
down uniform requirements of structures for the storage of liquids giving
due consideration to these factors. In order to fulfil this need, formulation
of this Indian Standard code of practice for concrete structures for the
storage of liquids [ IS : 3370-1965 J was undertaken. This part deals
with general requirements. Three other parts of the code are the
Part II Reinforced concrete structures
Part III Prestressed concrete structures
Part IV Design tables
0.3 Although the provisions of this code cover mainly structures for the
storage of liquids the general provisions of this code may also be applied
with such modifications as foun’d necessary, to suit the special conditions in
the design of reinforced concrete and prestressed concrete structures for
the conveyance of liquids, such as aqueducts and superpassages.
0.4 While the common methods of design and construction have-been
covered in this code, design of structures of special forms or in unusual
circumstances should be left to the judgement of the engineer and in such
cases special systems ofdesign and construction may be permitted on pro-
duction of satisfactory evidence regarding their adequacy and safety by
analysis or test or by both.
0.5 In this standard it has been assumed that the design of liquid retaining
structures, whether of plain, reinforced or prestressed concrete is entrusted
to a qualified engineer and that the execution of the work is carried out
under the direction of an experienced supervisor.
0.6 All requirements of IS : 456-1964* and IS : 1343-1960t, in so far as
they .apply, shall be deemed to form part of this code except where other-
wise laid down in this code.
0.7 The figures 1 to 7 given in this code are only diagramatic and are
intended merely to illustrate the definitions and principles given in the code
and need not be treated as preferred designs.
0.8, The Sectional Committee responsible for the preparation of this
standard has taken into consideration the views of engineers and technolo-
gists and has relatid the standard to the practices followed in the country
in this field. Due weightage has also been given to the need for interna-
tional co-ordination between the standards prevailing in different countries
of the world. These considerations led the Sectional Committee to derive
assistance from published materials of the following organizations:
British Standards Institution,
Portland CemeTt Association, Chicago, hSA, and
Institution of Civil Engineers, London.
0.9 For the purpose of decid,ing whether a particular requirement of this
standard is complied with, tHe final value, observed.,or cal+.dated, expres-
sing the result of a test or analysis, shall be rounded off in accordance
with IS : 2-1960$. The number of significatit places retained in the
rounded off value shw)d be the same as that of the specified value in this
1.1 This standard ( Part I) lays down the general requirements for the
&sign and construction of concrete structures, plain, reinforced or pres-
tressed concrete, intended for storage of liquids, mainly water.
The requirements applicable specifically to reinforced concrete liquid
retaining structures are covered in Part II.
*Code of practice for plain and reinforced concrete (secondrevision).
tCode of practice for prestressed concrete.
$Rules for rounding off numerical values ( rcmksd).
1.2 This code does not cover the requirements for reinforced and
tressed concrete structures for storage of hot liquids and liquids o low
viscosity and high penetrating power like petrol, diesel oil etc. Special
problems of shrinkage arising in the storage of non-aqueous liquids and the
measures necessary where chemical attack is possible, are also not dealt
with. The recdmmendations, however, may generally be applicable to
the storage at normal temperatures of aqueous liquids and solutions which
have no deterimental actiofi on concrete and steel or where sufficient
precautions are taken to ensure protection of concrete and steel from
damage due to action of such liquids as in the case of sewage.
2.1 The requirements for materials shall be governed by 4 of
IS : 4X-1964* and 4 of IS : 1343-1960t for reinforced concrete and pres-
tressed concrete members, respectively, with the following additional
Porousaggre.gates- Under no circumstances shall the use of porous
aggregates, such as burnt clay and broken brick’ or tile, be
allowed for parts of structure either in contact with the liquids
on any face or enclosing the space above the liquid.
Prestressing steel - The prestressing steel for prestressed concrete
members of the structure shall comply with the requirements of
either IS : 1785-1961f. or IS : 2090-1962s.
2.2 Jointing Materials -Joint, fillers, joint sealing compounds, water
bars and joint cover plates shall conform to the requirements of relevant
3. CONCRETE MIX
3.1 Provisions in 5 of IS : 456-1964* and 4.2.5 of IS : 1343-1960t shall
apply for reinforced concrete and prestressed concrete members, respecti-
vely, subject to the following further requirements:
a) Except in case of thick sections as described in 7 and parts of
structure neither in contact with the liquid on any face nor
enclosing the space above the liquid, concrete mix weaker than.
M 20dshall not be used.
*Code of practice for plain and reinforced concrete ( secondr~i~ion).
tCode of practice for prestressedconcrete.
$Spccificationfor plain hard drawn steel wire for pretrcsscd concrctc. ( Sincerevised
and splitinto two parts ).
$Spccilicationfor high tensilesteel bars used in prestremd concrete.
IS : 3370 ( Part I ) - 1965
b) The minimum quantity of cement in the concrete mix shall be
not less than 330 kg/ms in reinforced concrete work, 360 kg/m*
in post tensioned prestressed work and 380 kg/m3 in pretensioned
prestressed work. The maximum quantity of cement in the
concrete mix shall preferably not exceed 530 kg/ma of concrete.
c) The design of the mix shall be such that the resultant concrete
is sufficiently impervious. The mix obtained in accordance with
the above, if fuIly compacted, will generally give a degree of
impermeability adequate for all ordinary purposes. In special
circumstances, the engineer-in-charge should satisfy himself that
an adequate permeability is obtained by percolation tests.
3.2 Pneumatic Mortar
3.2.1 The grading of fine aggregates for pneumatic mortar should con-
form in general to grading zone I or II specified in Table 3 of
IS : 383-1963*.
NOTE -Pneumatic mortar is mortar applied pneumaticalIy through a suitable
nozzle; it is used, for example, as cover to external prestrcssingsteel. A- qqinternal
3.2.2 The proportions of pneumatic mortar should be such that the
ratio ( by weight) of cement content to fine aggregate is neither less than
(~3 nor more than 0.5.
3.2.3 A suitable mix for final cover coat of pneumatic mortar is 50 kg
cement, 4.5 kg hydrated lime and 140 kg of dry sand of such size that it
will pass through 2.36 mm IS Sieve.
3.3 Imperviousness of Concrete Mix - In the construction of concrete
structures for the storage of liquids, the imperviousness of concrete is an
important basic requirement. The permeability of any uniform and
thoroughly compacted concrete of given mix proportions is very largely
dependent on the water-cement ratio. While an increase in this ratio
leads to an increase in the inherent permeability, a very much reduced
water-cement ratio of a mix with a given cement content may cause compac-
tion difficulties and thus may prove equally harmful. For a given mix
made with particular materials, there is a lower limit to the water-cement
ratio which can be used economically on any job. It is essential to select
a richness of mix compatible with available aggregates, whose particle
shape and grading have an important bearing on workability which must
be suited to the means of compaction selected. Efficient compaction
prefer&ly by vibration is essential. In practice, it is usually convenient,
particularly when dealing with thin congested reinforced sections, to specify
a cement content sufficiently high to ensure that thorough compaction is
obtainable while maintaining a sllficiently low water-cement ratio. In
*Specificationfor coarseand fine aggregatefromnaturalsourcesfor concrete(r&red).
(Since revised 1.
thicker sections, where a reduction in cement content might be desirable to
restrict the temperature rise due to cement hydration, a lower cement
content is usually permissible, partly because the overall permeability of
~ the section is reduced by the greater thickness and partly because less
congested conditions may permit thorough compaction of a somewhat
While proper attention must be paid in achieving-a mix of inherently
low permeability, it should be recognized that common and more serious
causes of leakage in practice, other than cracking, are defects such as
segregation and honey combing and in particular all joints are potential
source of leakage.
The mixes as specified in 3, if fully compacted, will give a degree of
permeability adequate for all ordinary purposes. In special circumstances,
where necessary, the engineer should satisfy himself by a percolation test,
that an adequate degree of impermeability is obtained.
4. SI’I’F, CONDITIONS
4.1 The following conditions of the site in relation to the functional and
structural requirements of the liquid retaining ( storage ) structure materi-
ally influence the methods of design and the cost of the structure:
a) Physical characteristics of soil in which the liquid retaining
structure may be partly or wholly enclosed and also the physical
and geological features of the supporting foundations,
b) Extent of water-logging at the site, and
c) Chemical properties of the soil and of the ground water.
4.2 In making the choice of the site and in the preparation of the design
the factors mentioned in 4.1 should be taken into account generally as
Exfemal eurfhpr.~~e - Relief from external earth pressures either
wholly or partially should not generally be relied upon, unless
the operation of such pressures throughout the service life of the
liquid retaining structure is ensured. On the other hand, walls of
the liquid retaining structure shall be checked for external
pressures under empty or partially-empty conditions.
Water-logged ground - If in the sitting of a liquid retaining
structure, water-logged ground cannot be avoided, the dangers
of the external water pressure shall be carefully guarded against
the following: *
Designing the structure to resist such pressure under empty or
partially-empty conditions and taking precautions to prevent
floating and ensuring stable equilibrium under all conditions
of internal and external loads. It is advisable to make the
design such that the ‘minimum gravity weight exceeds the
uplift pressure by at least 20 percent.
Providing under Boor drainage to reduce the level of the
external water as far as local conditions permit.
Providing relief valves discharging into the liquid retaining
structure when the external .pressure exceeds the internal
pressure; this arrangement is feasible only in cases when the
liquid retaining structure is not required for the storage of
liquids which should not be contaminated.
Designing both internal and external faces of the walls and
tloor as water retaining faces, where the walls and floors of
the liquid retaining structure are submerged in water or
water bearing soils.
Stability- The equilibrium and safety of structure and parts of
it against sliding and overturning especially when the structure
is founded on a side long or sloping ground, shall also be checked.
Sttthnent and subsidence- Geological faults, mining, earthquakes,
existence of subsoils of varying bearing capacities may give rise,
to movement or subsidence of supporting strata which may result
in serious cracking of structure. Special considerations should
be given in the preparation of the design, to the possible effect
of subsidence or movement of the foundation strata.
Injurioussoils- Chemical analysis of the soil anu ground water is
essential in cases where injurious soils are expected to exist, as
concrete structure may suffer severe damage in contact with such
soils. The use of sulphate resisting cement will increase the
resistance to the action of certain injurious soils but may not
afford complete safeguard. An isolating coat of bituminous or
other suitable material may improve the protective measures.
5. PROTECYMON AGAlNST' CZORROSION
5.1 The type of liquid to be retained should be considered in relation to
the possibility of corrosion of steel or attack on concrete with corrosion
waters ( as in the case with certain natural waters ), it is desirable to use
richer and denser concrete and provide increased cover to steel. Consi-
derations may also be given to the use of special cements, such as,
sulphate-resisting cement or high alumina cement. Where attack is likely
to be appreciable the provision of an impervious protective lining should
6. CONTROL OF CRACKING
6.1 Design of liquid retaining structures has to be based on the avoidance
of cracking in the concrete having regard to its tensile strength. Important
causes of cracking in concrete and measures to be adopted for avoiding
them are given below.
6.1.1 Design of reinforced concrete members shouId be made in accor-
dance with the usual principle of ignoring the tensile resistance of concrete.
Additionally, it should also be ensured that the calculated tensile stress on
the liquid retaining face of the equivalent concrete section ( after allowing
for the steel area in equivalent concrete units) does not exceed the limits
prescribed by this standard [ JCCTable 1 of IS : 3370 ( Part II ) - 1965’ ]
assuming in the calculations that the entire section of the concrete ( includ-
ing cover) participates in resisting the direct and flexural loads. The
permissible limits of tensile stress in the concrete fGrcalculations relating to
resistance to cracking will naturally provide a much smaller margin of
safety against ultimate tensile strength of concrete because the consequences
of cracking are usually much less serious than those of structural failure.
In members less than 225 mm thick, the requirement of limiting’ the
tensile stress as given in 6.1.1 shall also be applied to the face remote from
the water retaining face.
6.1.2 Plain concrete liquid retaining structures or members may be
designed against structural failure by allowing tension in plain concrete as
per the permissible limits for tension in bending specified in IS : 456-1964t.
This will automatically take care of failure due to cracking. However,
nominal reinforcement in accordance with the requirements of
IS : 456-1964t shall be provided for plain concrete structural members.
6.1.3 The design of prestressed concrete members is based upon ’ no
tension ’ being developed in the concrete section under service conditions.
The design of prestressed concrete shall however be further checked against
cracking of the liquid retaining face with a load factor against cracking
_r* n01 1.4.
6.1.4 Cracking may also result from the restraint to shrinkage, free
expansion and contraction of concrete due to temperature and shrinking
and swelling due to moisture effects. Such restraint may arise from:
a) the interaction between reinforcement and concrete during drying
b) the boundary conditions at the foundations or other parts of the
c) the differential conditions through the large thickness of massive
concrete. Some of the methods employed to control or prevent
such cracking are given in 18.104.22.168 to 22.214.171.124.
*Codeof practicefor concretestructuresfor the storage of liquids, Part II Rrinforccd
tCcde of practiceforplainand reinforcedconcrete( second revision ),
IS : 3370( Part I ) - 1965
126.96.36.199 Correct placing of reinforcement, use of small sized bars and
use of deformed bars lead to a difused distribution of cracks.
188.8.131.52 The risk of cracking due to overall temperature and shrinkage
effectsmay be.minimized by limiting the changes in moisture content and
temperature to which the structure as a whole is subjected. Underground
reservoirs can remain permanently wet. It will be advantageous if during
construction of such reservoirs thin sections below final water level could
be kept permanently damp. It will, however, be impracticable to main-
tain permanent wetness in elevated structures which unavoidably may be
left empty for a period.
184.108.40.206 Cracks can be prevented in thick walls ( or even in thinner
sections) by avoiding the use of thick timber shuttering which prevent the
easy escape of the heat of hydration from the concrete mass. Due to such
heat of hydration, the concrete wall is raised to a relatively high tempera-
ture which will be retained during the period the concrete hardens. On
removaIc&he form work, as the temperature of concrete falls to that of the
surrounding air, the concrete contracts. Such contraction will take place
without cracking if the free movement of the wall is unrestricted, but cracks
may subsequently develop where one or more of the edges are restrained.
220.127.116.11 The risk of cracking can also be minimized by reducing the
restraints on the free expansion or contraction of the structure. With long
walls or slab; founded at or below ground level, restraints can be
minimized by the provision of a sliding layer. This can be provided by
founding the structure on a flat layer of concrete (see Note ) with inter-
position of some material to break the bond and facilitate movement.
However, the length of the wall that can be kept free of cracks by the use
of a sliding lajier in its foundation is .strictly limited and is related to the
tensile strength of the wall section. In approximate terms, the tensile
strength has to be sufficient to overcome the resistance to sliding of one
half of the length of the wall. Control of cracking thus requires sub-
division of the structure into suitable lengths separated by movement joints.
The maximum length desirable between joints will depend on the tensile
strength of the wall and mav be increased by suitable reinforcement. The
effectiveness of movement joints in controlling cracking will depend not
only on their spacing but often on their precise location. This is a matter
of experience and may be characterized as the place where cracks would
otherwise develop, for example, at changes of section. The location of al!
movement joints should be indicated on the drawings.
NOTE -In normal circumstances this flat lsycr of concrete may be weaker than that
used in other parts of the structure, but not weaker than M 100 specified in
IS : 456-19645. Where, however injurious soils or agressive ground water are expected,
the concrete should not be weaker than M 150 specified in IS : 456-1964*, and if
necessary a sulphate resisting or other special cempnt should b used.
*Code of practice for plain and reinforced concrete ( secondrrvirian ).
18.104.22.168 Where reservoirs are used for reception or storage of hot
liquids, allowance should be made for the additional stresses produced by
difference in temperature between inside and outside of the reservoir. The
severity of the temperature gradient through the concrete can sometimes be
reduced by internal insulation.
22.214.171.124 Whenever development of cracks or overstressing of the
concrete in tension cannot be avoided, the concrete section shoukl be
suitably strengthened. In making the calculations either for ascertaining
the expected expansion or contraction or for strengthening the concrete
section, the following values of the coefficient of expansion due to tempera-
ture and coefficient of shrinkage may be adopted:
Coefficient of expansion 11 X IO-‘/%
Coefficient of shrinkage initial shrinkage on first drying
450 x 10-s of the original length;
drying shrinkage 200 x 10e6 of the
6.2 Sustained stresses due to temperature and shrinkage effects may be
modified by ‘the occurrence of creep. This is often advantageous, for
instance, if the reservoir is filled at a slow rate ( a procedure which is
usually adonted ) the margin of safety against cracking may be increased
by the occur tence of creep. This procedure also has the advantage that
resaturatlon of the concrete before it is fully loaded will reduce the contri-
b&on which drying shrinkage might make to the formation of cracks.
6.3 Where reservoirs are protected with an internal impermeable lining,
the requirement that all cracking of the concrete be avoided should be
retained unless it is established on the basis of tests or experience that the
lining has adequate crack bridging properties.
7. THICK SECTIONS
7.1 Thick sections shall be those parts of structure which have thickness
greater than 450 mm. There is a likelihood of cracking in such sections as a
consequence of temperature rise during hydration of the cement and
subsequent cooling. Such cracking is not easy to control by reinforcement.
The following are some of the measures that may be adopted for reducing
the likelihood of cracking:
a) Magnitude of the temperature rise should be restricted by limiting
the cement content, or by using a type of cement with a low rate
of heat of evolution or adopting suitable construction methods;
Portland cements with lower rates or strength development
generally give lower rates of heat evolution. In such cases the
permissible stresses shall conform to requirements of 3.3. Tem-
perature rise may also be restricted by casting the concrete in ,-
shallow lifts at .intervals of a few days so as to allow the escape qf
part of heat from the exposed upper surface.
b) Steep temperature grading will occur by sudden chilling of the
concrete surface. This should be avoided, for instance, some
protection may be required when removal of heavy timber form-
work coincides with on set of cold weather.
c) Restraint to overall contraction may be limited by provision of
movement joints and by provision of suitable sliding layer
( see126.96.36.199 and 188.8.131.52 ). Another cause of restraint which may
lead to cracking occurs when a substantial lift of concrete is cast
upon a cold foundation. A better procedure is to avoid excessive
disparity in temperature between successive lifts and where prac-
ticable to introduce shallow lifts when starting from or resuming
work on a cold foundation.
‘I.!2 While concreting in thick sections, the requirements of IS : 456-196P
shall apply as far as possible.
8.1 Joints shall be categorized as below:
a) Movetnent Joints - There are three categories of movement joints:
Cfmtracfionjoint - A movement joint with a deliberate discon-
tinuity but no initial gap between the concrete on either side
of the joint, the joint being intended to accommodate contrac-
tion of the concrete ( seeFig. 1 ).
A distinction should be made between a complete
contraction joint (see Fig. 1A ) in which both concrete and
reinforcing steel are interrupted, and a partial contraction
joint (.seeFig. 1B ) in which only the concrete is interrupted,
the lemforcing steel running through.
Expa&m joint - A movement joint with complete discontinuity
in both reinforcement and concrete and intended to accom-
modate either expansion or contraction of the structure
(see Pig. 2).
In general, such a joint requires the provisron of an
initial gap between the adjoining parts of a structure which by
closing or opening accommodates the expansion or contraction
of the structure. Design of the joint so as to incorporate
sliding surfaces, is not, however, precluded and may some
times be advantageous.
CONCRETE BUT NO JOINT SEALING
INITIAL GAP ,-WATER BAR COMPOUND- ,,&lRIP PAINTING
IA Complete Contraction Joint
FIO. 1 TYPICAL
CONCRETE BUT NO
1B Partial Contraction Joint
WATER BAR- It-INITIAL GAP
LYDISCONTINUITY IN BOTH
CONCRETE AND STEEL
Fm 2 A TYPIOAL FXPANSIONJOINT
3) Sliding joint - A movement joint with complete discontinuity
in both reinforcement and concrete at which special provision
is made to facilitate relative movement in place of the joint.
A typical application is between wall and floor in some
cylindrical tank designs ( se@Fig. 3 ).
b) Construction Joint-A joint in the concrete introduced for
convenience iri construction at which special measures are taken
to achieve subsequent continuity without provision for further
relative movement, is called a construction joint. A typical
application is between successive lifts in a reservoir w@l
(see Fig. 4).
OR RUBBER PAD
FIG. 3 A TYPICAL SLILXNOJOINT
Fxo. 4 A TYPICAL CONSTIKJCTIONJOINT
The position and arrangement of all construction joints
should be predetermined by the engineer. Consideration should
be given to limiting the number of such joints and to keeping
them free from possibility of percolations in a similar manner to
Temprary Open Joints - A gap temporarily left between the con-
crete of adjoining parts of a structure which after a suitable
interval and before the structure is put into use, is filled with
mortar or concrete either completely ( Fig. 5A) or as provided
below, with the inclusion of suitable jointing materials ( Fig. 5B
and SC). In the former case the width of the gap should be
sufficient to allow the sides to be prepared before filling.
Where measures are taken for example, by the inclusion of
suitable jointing materials to maintain the watertightness of the
concrete subsequent to the filling of the joint, this type of joint
may be regarded as being equivalent to a contraction joint
( partial or complete ) as defined above.
8.2 Design of Joints -Design of a movement joint should aim at the
following desirable properties for its efficient functioning:
a) The joint should accommodate repeated movement of the struc-
ture without loss of watertightness.
INITIAL GAP LATER
FILLED WITH CONCRETE
INlTIAL GAP LAlER
INIT STRIP PAINTING
JOINT SEALING C
Fm. 5 TYPXCAL TEMPORARY OPEN JOINTS
b) The design should provide for exclusion of grit and debris which
would prevent the closing of the joint.
c) The material used in the construction of movement joints~should
have the following properties:
1) it should not suffer permanent dutortion or extrusion and
should not be displaced by fluid pressure.
2) it should not slump unduly in hot weather or become brittle
in cold weather.
3) it should be insoluble and durable and should not be affected
by exposure to light or by evaporation of solvent or
4) in special cases, the materials should be non-toxic, taintless or
resistant to chemical and biological action as may be specified.
8.3 Spacing of Joints - Unless alternative effective means are taken to
avoid cracks by>allowirng for the additional stresses that may be induced by
temperature or shrinkage changes or by unequal settlement, movement
joints should be provided at the following spacings:
a) In reinforcement concrete floors, movement joints should be
spaced at not more than 7*5 m apart in two dirbions at right
IS? 3370 ( Part I) - 1965
angles. The wall and floor joints should be in line except where
shdmg joints occur at the base of the wall in which case corres-
pondence is not so important.
For, floors with only nominal percentage of reinforcement ( smaller
than’fhe minimum specified ), the concrete floor should be cast iid
panels with sides not more than 4.5 m.
In concrete walls, the vertical movement joints should normally
be placed at a maximum spacing of 75 m in reinforced walls and
6 m in unreinforced walls. The maximum length desirable
between vertical movement joints will depend upon the tensile
strength ,of the walls, aqd may be increased by suitable reinforce-
ment. Thus when a shding layer is placed at the foundation ofa
wall, the length of wall that can be kept free of cracks depends
upon the capacity of wallsection to resist the friction induced at
the plane of sliding. Approximately the wall has to stand the
effect of a force at the plane of sliding equal to weight of half the
length of wall multiplied by the coefficient of friction.
Amongst the movement joints in floors and walls as mentioned
above, expansion joints should normally be provided at a spacing
of not more than 30 m between successive expansion joiitts or
between the end of the structure and the next expansion joint+11
other joints being of the contraction type.
When, however, the temperature changes to be accommodated
are abnormal or occur more frequently than usual as in the case
of storage of warm liquids or in uninsulated roof slabs, a smaller
spacing than 30 m should be adopted, ( that is a greater propor-
tion of the movement joints should be of the expansion type )
When the range of temperature is small, for example, in certain
covered structures, or where restraint is small, for example, in
certain elevated structures none of the movement joints provided
in small structures upto 45 m length need be of the expansion
type. Where sliding joints are provided between the walls and
either the floor or roof, the provision of movement joints in each
element can be considered independently.
8.4 Malsing of Joints -Joints shall gtarerally be made according to the
broad principles discussed in 8.4.1 to 8.4.3.
8.4.1 Construction Jo&t, -These should be set at right angles to the
general direction of the member ( seel&g. 4 ). The position and arrange-
men4 of construction joints should be determined by the engineer at the
de&ign stage and indicated on the drawings.
The surface film of the first-placed concrete should preferably be
rcmov?d whilst the concrete is still green to expose the aggregate and leave
a sound irregular surface. This may be eRected by spraying with water, -
or air and water, assisted by light brushing, where necessary. If the con-
crete has been allowed to harden, it will be necessary to achieve the desired
surface by hacking the whole of the surface, care being taken to avoid
damaging the aggregate.
While the remainder of the concrete should be kept continuously wet,
curing of the joint surface may be suspended a few hours before concreting
is to be resumed so as to permit no more than superficial drying of the
joint surface. Just before concreting is resumed, the roughened joint
surface should be thoroughly cleaned and freed from loose matter, pre-
ferably, without re-wetting, and then treated with a thin layer of cement
grout, worked well into the surface, or treated with cement/sand mortar in
which water/cement and sand/cement ratios do not exceed those in the
new concrete. Special care should be takec to avoid segregation of the
concrete along the joint plane and to obtain thorough compaction.
Alternatively, for horizontal joints the layer of grout or mortar may
be omitted, provided that the workability offirst batches of concrete placed
in contact with the joint is slightly increased.
8.4.2 Movement Joints - These require the incorporation of special
materials in order to maintain watertightness whilst accommodating rela-
tive movement between the sides of the joint. Suitable materials for this
purpose are referred to in 8.5.
Movement joints, particularly those in floor and roof, also require
protection against the entry of debris which may interfere with the closing
of the joints.
184.108.40.206 Contrilction joints - The joints face of the first-cast concrete
should be finished against a stopping-off board, or vertical end shutter,
which, in the case of a partial contraction joint, should be notched to pass
Steps should be taken to prevent any. appreciable adhesion between
the new and the old concrete.
The joint should be suitably treated so as to maintain watertightness
during movement of the joint ( see Fig. E and 8.5)
8.4.2.i Expansion joints - These require the provision of an initial gap
between the concrete faces on the two sides of the joint and this can be
conveniently done by the use of materials discussed in 8.5. The initial
width of this gap should be specified by the engineer and should be suffi-
cient to accommodate freely the maximum expansion of the structure. In
determining the initial width, regard should be paid to the requirements ~
of the jointing materials. These will normally require the maintenance of
a certain minimum width of gap during maximum expansion of the /
T METALLIC WATER BAR
TWO COAT STRIP
MOULDED WATER BAR
FIG. 6 TYPICAL DETA’LLBSROWINCZUSE OB JOINTINQ MATEBIALB TN
MOVEMENT JOINTB ( GINTIZACTION TYPE )
structure. The joint should be suitably treated so as to maintain water-
tightness during movement of the joint ( sod8.5 and Fig. 7 ).
220.127.116.11 Sliding joints
be plane and smooth.
- The two concrete faces of a sliding joint should
Care should be taken by the use of a rigid screeding board or other
suitable means to make the top of the lower concrete as flat as possible.
This surface can usefully be improved by finishing with a steel float and
rubbing down with Carborundum.
Bond between the concrete of the two components should be preven-
ted by painting or by inserting building paper or other suitable material.
The joint should be suitably treated so as to maintain watertightness
during movement of the joint.
8.4.3 Temporary Open Joints - The concrete on both sides of the joints
Aould be finished against stopping off boards.
+lETALLIC WATER BAR
f RUBBER WATER BAR
SHEET LEAD JOINT
PAINT-/ /- JOINT FILLER
/-JOlNT SEALING COMPOUND
rCOPPER JOINT COVER PLATE
L‘cl PLATE CAST LJ~NT FILLER
TWO COAT STRIP
7E STRIP PAINTING
Fro. 7 TEIOAL DXTAILE SHOWIH~ USE or JOINTR?G MATERI- IN MOVXMENT
In order to minimize the extent of subsequent movements due to
shrinkage the joint should be left open until shortly before the reservoir is
put into service and then filled in with mortar or concrete of specified
ture is low.
Where possible, the joint should be filled when the tempera-
Immediatly before filling the gap, the joint faces should, if possible,
be thoroughly cleaned and prepared in the same way as for construction
joints ( see8.4.1).
Where it is intended to treat this type of joint as equivalent to a
contraction joint for the purpose of this code, the joint should be suitably
sealed so as to maintain watertightness during subsequent movement of
85 Jointing Materials -Jointing materials may be classified as follows:
a) Joint fillers,
b) Water bars and joint cover plates, and
c) Joint sealing compounds ( including primers where required ).
8.5.1 Jo& Fillers-Joint fillers are usually compressible sheet or strip
materials used as spacers. They are fixed to the face of the first placed
concrete and against which the second placed concrete is cast. With an
initial gap of about 30 mm, the maximum expansion or contraction that
the filler materials may allow may be of the order of 10 mm.
Joint fillers, as at present available, cannot by themselves function
as watertight expansion joints. They may be used as support for an
effective joint scaling compound in floor and roof joints. But they can
only be relied upon as spacers to provide the gap in an expansion joint,
the gap being bridged by a water bar ( seeFig. 7 ).
85.2 Wafer Bars -Water bars are preformed strips of impermeable
material which are embeded in the concrete during construction so as to
span across the joint and provide a permanent watertight seal during the
whole range of joint movement. The most usual forms of water bars are
strip with a central longitudinal corrugation ( see Fig. 6A and 7A ),
Z shaped strip ( seeFig. 7B ), and a central longitudinal hollow tube ( see
Fig. 6B and 7C ) with thin walls with stiff wings of about 150 mm width.
The material used for the water bars are copper bars, sheet lead, natural
or synthetic rubbers ( seeFig. 7C ) and plastics such as polyvinyl chloride
( PVC ) ( seeFig. 6B ). Galvanized iron sheets may also be used with the
specific permission of the engineer-in-charge provided the liquids stored or
the atmosphere around the liquid retaining structure is not excessively
corrosive, for example, sewage.
Of the metals available copper is most suitable for use aswater bar as
regards ductivity and resistance to corrosion in air, water and concrete.
It may, however, be attacked by some wastes. If sheet lead is used, it
should be insulated from concrete by a good coat of bituminous or suitable
composition. Natural and synthetic rubbers and plastics have very consi-
5 derable advantage in handling, splicing and in making intersections.
With all water bars, it is important to ensure proper compaction of
the concrete. The bar should have such shape and width that the water
path through the concrete round the bar should not be unduly short.
The holes sometimes provided on the wings of copper water bars to
increase bond shorten the water path and may be disadvantageous. The
water bar should either be placed central* in the thicknessof the wall or
its distance from either face of the wall should not be less than half the
width of the bar. The full concrete cover to all reinforcement should be
The strip water bars at present available in the newer materials need
to be passed through the end shutter of the first-placed concrete. It cau
be appreciated, however, that the use of the newer materials make possible
a variety of shapes or sections. Some of these designs, for example, those
with several projections (see Fig. 6D ), would not need to be p&
through the end shutter and by occupying a bigger proportion of the
thickness of the joint would also lengthen the shortest alternative water
path through the concrete.
8.5.3 Joint Cover Plates -Joint cover plates are sometimes used in
expansion joints to avoid the risk of a fault in an embedded water-bar.
The cover plate may be of copper or sheet lead. If copper cover plate is
used it should be clamped to the concrete .face on each side of the joint
using suitable gaskets to e&u-e watertightness (me Fig. 70). If sheet
lead is used, the edges may return into grooves formed in the concrete and
be made completely watertight by lead caulking (see Fig. 7E). Faces of
the concrete to which sheet lead is to be fixed should be painted with bitu-
minous or other suitable composition and the lead sheet should be similarly
coated before fixing.
8.5.4 Joint Sealing Compounds -Joint sealing compounds are imper-
meable ductile materials which are required to provide a watertight seal
byadhesion to the concrete throughout the range of joint movement. The
commonly used materials are based on asphalt, bitumen, or coal tar pitch
with or without fillers, such as lime stone or slate dust, asbestos fibre,
chopped hemp, rubber or other suitable mater;?!. “rhese are usually
applied after construction or just before the reservoir is put into service by
pouring in the hot or cold state, by trowelling or gunning or as preformed
strips ironed into position. These may also be applied during construction
such as by packing round the corrugation of a water bar. A primer is often
used to assist adhesion and some local drying of the concrete surface with
the help of a blow .lamp is advisable. The length of the shortest water..
IS:3370(Part I)- 1965
path through the concrete should be, extended by suitably painting the
surface of the concrete on either side of the joint.
The main difficulties experienced with this class of material are in
obtaining permanent adhesion to the concrete during movement of the
joint whilst at the same time ensuring that the material does not slump or
is not extruded from the joint.
In floor joints, the sealing compound is usually applied in a chase
formed in the’ surface of the concrete along the line of the joint (see
Fig. 7C ). The actual minimum width will depend on the known charac-
teristics of the material. In the case of an expansion joint, the lower part
of the joint is occupied by a joint filler ( seeFig. 7F ). This type of joint is
generally quite successful since retention of the material is assisted by
gravity and, in many cases, sealing can be delayed until just before the
reservoir is put into service so that the amount ofjoint opening subsequently
to be accommodated is quite small. The chase should not be too narrow
or too deep to hinder complete filling and the length of the shortest water
path through the concrete should be extended by suitably painting the
surface of the concrete on either side of the joint. Here again a wider
joint demands a smaller percentage distortion in the material.
An arrangement inc&porating a cover slab, similar to that shown in
Fig. 7G, may be advantageous in reducing dependence on the adhesion of
the sealing compound in direct tension.
Using of sealing compounds for vertical joints is not very successful.
A stepped-joint instead of a straight through-joint with a water bar incor-
porated in the joint and sealing compound packed round the corrugation
of the water bar would be much more successful.
9.0 Unless otherwise specified in this code, and subject to the following
additional recommendations, the provisions of IS : 456-1964* and
IS : 1343-1960t shall apply to the construction of reinforced concrete and
prestressed concrete liquid retaining structures, respectively.
9.1 Thick Sections-The precautions necessary in the construction of
thick sections shall be observed as per requirements of 7.
9.2 Joints -Joints shall be constructed in accordance with requirements
9.3 Mixing and Placing of Pneumatic Mortar
9.3.XMixing -The aggregate and cement should be mixed in an
approved mechanical mixer and delivered from an approved mechanical
*Codeofpracticeforplainand reinforced concrete ( second revision ).
*Code of practiceforprestressedconcrete.
digester. The minimum amount of water should be injected into the
mixture as this will ensure maximum density of the mortar.
9.3.2 Placing -The pneumatic mortar should be applied with an
approved nozzle by a skilled operator. ..The velocity of the material leav-
ing’ the nozzle should be maintained uniform and should be such as to
produce minimum rebound of sand.
9.3.3 Cuting - Immediately after pneumatic mortar has been placed it
should be protected against premature drying by shading from strong
sunshine and shielding from the wind. As soon as it has hardened just
sufficiently to avoid damzge it should be thoroughly wetted and thereafter
kept wet continuously for at least seven days. Adequate protection
against fluctuations in temperature by shading and shielding, shall also
9.4 Construction of Floors
9.4.1 Floors Founded on the Ground
S.4.1.1 The ground should be covered with an at least 75 mm thick
plain concrete screed of composition as described in 18.104.22.168. Floors cast on
the ground should be in not less than two layers, the bottom layer of which
may comprise or replace the plain concrete screed. When the screeci forms
an integral part of the floor slab forming one of the two layers then the
mix for screed shall conform to the requirements of 3.
22.214.171.124 A layer of building paper or other suitable material should be
laid between successive layers.
126.96.36.199 The layers, other than the plain concrete screed, if used;
should be placed in panels, the sides of which should not exceed 7.5 m in
the case of reinforced slabs and 4.5 m in the case of plain slabs.
The tendency for the development of cracks in the upper layer of
paving slab or a reservoir Aoor is greatly diminished if the reinforcement is
discontinuous through the joints and it is recommended that the floor
panels be laid in chessboard fashion ( all the ‘ black ’ or a11the ‘ white ’
squares first ). The edges of the panels in the bottom layer may be butt-
jointed and the panels in the various layers should be arranged to break
9.4.2 Suspended Floors - Floors which are not directly supported on the
ground should be cast in panels, the sides of which should not exceed
7-5 m. At joints in suspended floors, the surface of the panels for a width
not less than the thickness of the panel on each side of the joint should be
primed and painted with at least two coats of bituminous or other approved
9.4.3 Junction of Floor and Walls -Where the wall is designed ‘to be
monolithic with the bottom slab, a suitable arrangement of reinforcement
and form-work shall be made to facilitate the form-work to fit tightly and
avoid leakage of cement paste from newly deposited concrete as such leak:
age if allowed to take place is very liable to cause porosity in the finished
concrete. One such arrangement is by providing a continuous upstand
section of the wall cast at the same time, as, and integrally with, the slab;
the height of this upstand must be sufficient to enable the next lift of
form-work to fit tightly and avoid leakage of the cement paste from the
newly deposited concrete.
9.5 construction of Walls
9.5.1 In all cases where the reinforcing steel is discontinuous at vertical
contraction joints, the walls should be constructed in alternate panels with
as long a pause as practicable before the concrete is placed in the interven-
9.5.2 Where the reinforcement is continuous through vertical joints in
walls, construction in alternate panels may result in a greater tendency to
the’ development of cracks in those panels which are cast between two
earlier placed panels, the existence of which increases restraint of the
natural shrinkage of the intermediate panel.
9.5.3 The height of any lift should not exceed 2 m unless special
precautions are taken to ensure through compaction throughout by
me&a&al vibration or by other suitable means.
9.5.) All vertical joints should extend the full height of the wall in un-
9.6 8Ivface Finish to Prastressed Concrete Cylindrical Tanks - The
circumferential prestressing wires of a cylindrical tank should be covered
with a protective coat, which may be pneumatic mortar, having a thick-
ness that will provide a minimum cover of 40 mm over the wires.
9.7.1 Removal of Formwork - The requirements shall conform to 29.2.3 of
IS : 456-1964*.
9.7.2 Bolts passing completely through liquid-retaining slabs for the
purpose of securing and aligning the form-work should not be used unless
effective precautions arc takerrto ensure water-tightness after removal.
9.8 Lining of Tanks .- The type of liquid to be stored should be consi-
dered in relation to the possibility, of corrosion of thesteel or attack on-the
*Code of practice for plain and reinforced concrete ( sand rmXon).
IS : 3370( Part I) - 1965
concrete. Provision of an impermeable protective lining should be consi-
dered for resistance to the effects of corrosive liquids. Certain natural
waters exhibit corrosive characteristics and in such cases it is important to
obtain a dense impermeable concrete and with a higher cement content.
An increased cover to the steel is also desirable. Use of sulphate resisting
portland cement, pozzolana cement, of blast-furnance slag cement may in
certain cases be advantageous.
10. TESTS ON STRUCTURE
10.1 In addition to the structural test of the structure, as given in 21.3 oi
IS : 456-1964*, the tanks shall also be tested for watertightness at full
supply level as described in 10.1.1, 10.1.2 and 10.1.3.
10.1.1 In the case of tanks whose external faces are exposed such as
elevated tanks, the requirements of the teSt shall be deemed to be satisfied
if the external faces show no signs of leakage and remain apparently dry
over the period of observation of seven days after allowing a seven day
period for absorption after filling.
10.1.2 In the case of tanks whose external faces are submerged and are
not accessible for inspection, such as underground tanks, the tanks shall be
filled with water and after the expiry of seven days after the filling, the
level of the surface of the water shall be recorded. The level of the water
shall be recorded again at subsequent intervals of 24 hours over a period
of seven days. The total drop in surface level over a period of seven days
shall be taken as an indication of the watertightness of the tank. The
engineer-in-charge shall decide on the actual permissible nature of this
drop in the surface level, taking into account whether the tanks are open
or closed and the corresponding effect it has on evaporation losses. For
many purposes, however, underground tanks whose top is covered may be
deemed to be water-tight if the total drop in the surface level over a period
of seven days does not exceed 40 mm.
10.1.3 If the structure does not satisfy the conditions of test, and the
daily drop in water level is decreasing, the period of test may be extended
for a further seven days and if specified limit is then reached, the structure
may be considered as satisfactory.
l Code of practiceforplain and reinforced concrete ( srcond misim ).
BUREAU OF INDIAN STAND,ARDS
Manak Bhrvan, 9 Bahadur Shah Zafar Marg, NEW DELHI 110002
Telephones : 331 01 31, 331 13 75 Telegrams : Manaksanrtha
( Common to all offices) ’
-Manak Bhavan, 9 Bshadur Shah Zafar Marg,
1/14 C.I.T. Scheme VI I M, V. I. P. Road,
Maniktola, CALCUTTA 700054
SC0 445-446, Sector 35-C,
331 01 31
Southern : C. I. T. Campus, MADRAS 600113
twestern : Manakalaya, E9 MIDC, Marol, Andheri (East),
‘Pushpak’ Nurmohamed Shaikh Marg, Khanpur,
SPeenya Industrial Area, 1st Stage, Bangalore Tumkur Road
Gangotri Complex, 5th Floor, Bhadbhada Road, T. T. Nagar,
Plot No. 82/83, Lewis Road, BHUBANESHWAR 751002
53/5, Ward No. 29, R. G. Barua Road, 5th Byelane,
5-8-56C L. N. Gupta Marg ( Nampally Station Road),
RI4 Yudhister Marg, C Scheme, JAIPUR 302005
1171418 B Sarvodaya Nagar, KAN PU R 208005
Patliputra Industrial Estate, PATNA 800013
T.C. No. 14/1421, University P.O., Palayam
inspection Off7ce (With Sale Point) :
Pushpanjali, 1st Floor, 205-A West High Court Road,
Shankar Nagar Square, NAGPUR 440010
Institution of Engineers ( India ) Building, 1332 Shivaji Nagar,
*Sales Offlce in Calcutta is at 5 Chowringher Approach, P-0. Prlncep
Street, Calcutta 700072
fSales Office in Bombay Is at Novelty Chambers, Grant Road,
*Sales Office in Bangalore Is at Unity Building, Narasimharaja Square
41 24 42
6 32 92 95
[ 263482 63 49
13838 4949 5556
5 36 27
3 31 77
6 98 32
21 68 76
21 82 92
6 23 05
2 51 71
27 66 00
89 65 26
22 36 71
AMENDMENT NO. 1 COTOBER 1982
ISd7D(Part I)-1965 CODE OF PRACTICE fOR CONCRETE
STRUCTURES FOR THE STORAGE OF LIQUIDS
PART I GENERAL REQUIREMENTS
(Page 3, oluu8e 0.3) - Substitute the following
for the existing clause:
'0.3 Although the provisions of this code cover mainly
3tructurer for the storage of liquids, the general
requirements given in Part I of this code my generally
apply to the design of reinforced concrete and
prestressed concrete structures for the conveyance
of liquids, such as aqueducts and superpassages;the
other requirements given in the code may also be applied
with appropriate modifications.'
(?age 6, ckxzaw 3.1, Zast line) - Substitute
'impermeability @F lpermeability'.
&$s 7s cZuu8e 3.3, t&e 13) - Substitute
Printed at Slmco Printing Press, Dell?-